Materials 2012, 5, 1247-1257; doi:10.3390/ma5071247
materials ISSN 1996-1944
Laser Treatment of Cotton Fabric for Durable Antibacterial Properties of Silver Nanoparticles
Shirin Nourbakhsh * and Ali Ashjaran
Textile Department, Shahre Rey Branch, Islamic Azad University, P.O. Box 18155-144, Tehran 001-680-000, Iran; E-Mail: [email protected]
Received: 14 March 2012; in revised form: 22 May 2012 / Accepted: 18 June 2012 / Published: 16 July 2012
Abstract: In the present study, cotton fabric was exposed to laser exposure at different energy levels and then the silver nanoparticles were coated on untreated and laser treated cotton fabrics. Methylene blue dye was used to detect the presence of carboxylic acid groups (-COO−) on laser treated cotton and the dye absorption results were determined spectrophotometrically. ICP-OES (Inductively Coupled Plasma Optical Emission Spectroscopy) analysis and antibacterial tests were carried out to investigate the silver ion content and bactericidal properties of silver nanoparticles on cotton fabrics. Infrared spectroscopy (FTIR/ATR) analysis and scanning electron microscopy (SEM) were used to identify chemical changes and to study the morphology of the surface of the fibers. EDAX (Energy Dispersive X-ray Spectroscopy) analysis was calculated for SEM micrographs. The results showed according to the higher uptake of methylene blue dye that the negative charge of the carboxylic acid groups had been created by laser treatment. Although the FTIR spectroscopy results did not show an increase in carboxylic acid groups, the cationic dye absorption increased. The durability of the Ag+ ion particles on repeated laundered laser treated cotton was proven by antibacterial and ICP tests, particularly when the laser energy was increased.
Keywords: laser ablation; silver nanoparticles; durability; cotton; antibacterial
Materials 2012, 5
The growth of microorganisms on textiles can cause problems, therefore, textile products are often treated with antimicrobial agents to prevent the proliferation of microorganisms [1,2]. Silver metal is one such antibacterial material which has been utilized for many years. A very low concentration of silver ions is sufficient for antibacterial effects. Silver nanoparticles have recently been used as a safe antibacterial agent for human health on different materials such as fibers, polymers and antimicrobial textile products. Durability of antimicrobial finishes on textiles is important for consumer usage. Research continues to find ways of increasing lasting antibacterial effects in the fabric. In this study, silver nanoparticles were applied on untreated and laser treated fabrics, the surface of which had been laser modified to investigate the durability of silver ions [3–9]. The cotton fiber consists of hydroxyl groups which are affected by chemical interactions. The hydroxyl groups are converted to carboxyl and carbonyl groups in the presence of oxidative agents or oxygen plasma discharge [10–14].
Laser is classified as light amplification by stimulated emission of radiation . The optimal characteristics of laser light have increased its application in many fields including medical, industrial, and the military. The benefit of laser is due to its high-speed, more handling safety and unique process applications. The laser used in the textile industry is of great importance and is used for the decoloration of denim [16–18], cutting fabrics in industry , and wool shrinkage control as laboratory work . There are several commercial lasers in industry, which are used for industrial applications, including, the laser of Nd:YAG, CO2 and Excimer . In previous works, coating of silver nitrate and silver nanoparticles on plasma treated and untreated cotton and cotton/polyester fabrics were investigated [3,20–25]. The researchers used silver nitrate and silver nano-particles to illustrate the higher absorption of silver ions on nitrogen plasma treated and cationized cotton fabrics [22,24]. In this study, the CO2 laser was used for surface modification of cotton fabrics and then the cotton fabrics were dyed by methylene blue dye for investigation of the existence of carboxylic acid groups. The Infrared spectroscopy analysis (FTIR/ATR) and scanning electron microscopy (SEM) were utilized to determine the functional groups and surface morphology. Silver nanoparticles were applied on untreated and laser treated cotton fabrics. ICP-OES analysis and anti-bacterial tests were obtained in accordance with the standard procedures and the laundering was repeated to determine the durability of anti-bacterial effects on cotton fabrics.
2. Results and Discussion
The color parameters (L*, a*, b*), K/S value (color yield) and ΔE (color difference) of dyed fabrics by methylene blue dye are indicated in Table 1. The methylene blue dye is a cationic dyestuff which reacts with anionic substrates and is used for determination of carboxylic acid groups on oxidized cotton . The L* value indicates the lightness of the dyed fabric and a lower amount of lightness means a darker fabric. The untreated cotton fabric showed an L* value of 70.45, and after laser treatment at a power of 1000 W, the L* value decreased to 69.87 and 69.05. The increase of applied laser energy on cotton fabrics caused the higher amount of methylene blue dye absorption due to the reduction of L* value. The color yield of the dyed fabrics is obtained from the following Kubelka-Munk Equation:
Materials 2012, 5
K/S = (1 − R)2/2R (1)
where R is the reflectance; the K/S value reveals the color yield of the dyed fabric. When the fabric becomes darker, the color yield increases. The color strength (K/S) for untreated cotton fabric was 0.636 and it increased to 0.782 and 0.832 for laser treated cotton fabric at a power of 100 watts and the fabric became darker. It seems that the laser effect at a power of 100 watts was significant for the absorption of cationic dye; this is due to the presence of anionic groups on the cotton surface which might be carboxylic acid groups. Color difference (ΔE) of untreated and laser treated cotton fabric is calculated by the Equation (2) :
222 baLE ∆+∆+∆=∆ (2)
Table 1. Color parameters of methylene blue dyed untreated and laser treated cotton fabric.
Power (w) 100 75 50 Untreated
Scan speed (cm/s) 1000 2000 1000 2000 1000 L* 69.05 69.87 70.16 70.11 70.41 70.45 A* −5.49 −5.53 −2.76 −4.58 −2.13 −2.38 B* −18.41 −18.18 −12.36 −7.45 −14.75 −16.09 K/S 0.832 0.782 0.731 0.651 0.648 0.636 ∆ E 4.12 3.82 3.76 2.6 1.36 –
The color difference of laser treated cotton fabrics was calculated as compared to untreated fabric. The color difference increased to 4.12 for laser treated cotton fabric at a high level of energy. The increase in laser power affected on dye absorption as the results of ΔE indicated.
In Figure 1 we can see the Ag ion content on untreated and laser treated cotton fabrics which were obtained by ICP-OES analysis. The untreated cotton fabric showed 0.024% of Ag ion content and it decreased to 0.009% after repeated laundering. The highest amount of observed silver ions was 0.047% for the higher energy level of laser (100 W, 1,000 cm/s) which reduced to 0.028% with repeated laundering. These results show that not only the laser effect and its higher energy level can increase the absorption of silver ions on cotton surface but also the durability of silver ions remained after repeated laundering.
Figure 1. The silver ion content on untreated and laser treated cotton fabrics.
Materials 2012, 5
Table 2 shows the percentage of bacteria reduction with silver nanoparticles on untreated and laser treated cotton fabrics. The antibacterial tests were performed with two kinds of bacteria; Escherichia- Coli and staphylococcus aureus. Results showed that the silver ion was more effective in reducing Escherichia coli than Staphylococcus aureus bacteria. By increasing the laser energy level, silver ion absorption increased on cotton fabric as the percentage of bacteria reduction reached 99.25% at 100 W and 1,000 cm/s laser conditions and after repeated laundering it decreased to 98.3%. Whereas a silver nanoparticles coating on untreated cotton fabric showed 39.9% of bacteria reduction. Figures 2 and 3 show the colonies of bacteria (E. coli and S. aureus) on untreated and laser treated cotton fabrics at 100 W and 1,000 cm/s. The colonies of bacteria were counted and the percentage of bacteria reduction was calculated using Equation (3).
Table 2. Bacteria reduction percentage, Ag content results of EDAX analysis of a silver nanoparticles coating and carboxyl groups’ contents of untreated and laser treated cotton fabrics.
Figure 2. The bacteria colonies of a silver nanoparticles coating on untreated cotton (a) Escherichia Coli before laundering; (b) Escherichia Coli after laundering; (c) Staphylococcus aureus before laundering; (d) Staphylococcus aureus after laundering.
(a) (b) (c) (d)
Bacteria Laser power (w) 100 75 50 Untreated Scan speed (cm/s) 1000 2000 1000 2000 1000
Escherichia Coli Before laundering 99.25 98.65 98.4 96.45 98.05 39.9 After laundering 98.3 97.45
Click here to load reader